australian asphalt pavement association crumb rubber modified 2018-06-29آ page | 2 crumb rubber...
Post on 30-Mar-2020
Embed Size (px)
Australian Asphalt Pavement Association
Crumb Rubber Modified Open Graded and Gap Graded Asphalt Pilot Specification _________________________________________________________________________________
Version: 1.0 12 June 2018
National Technology and Leadership Committee
This work is licensed under a Creative Commons Attribution 3.0 Australia License.
Page | 1 Crumb Rubber Modified Open Graded and Gap Graded Asphalt Pilot Specification
Preface This pilot specification is intended as a guide for asset owners in the creation of technical specifications for the supply of crumb rubber modified (CRM) open graded asphalt (OGA) and gap graded asphalt (GGA) mixes. The mixes contain a bituminous binder with partially digested crumb rubber (i.e. high-viscosity CRM binder). The crumb rubber modified binder technology in this specification is based on the technology used in California and Arizona. The CRM OGA mix design process in this specification has been validated through demonstration trials in Australia. The CRM GGA mix design process described in this specification is yet to be validated in Australia. The aim of this pilot specification is to facilitate the construction of demonstration trials of CRM GGA, as well as to promote the wider use of CRM OGA in Australia. The content of this specification builds on information in the following documents • Transport and Main Roads Specification PSTS112 Crumb Rubber Modified Open Graded
Asphalt Surfacing, Queensland Government, 2016 (not published). • National Asphalt Specification, 2nd edition, Australian Asphalt Pavement Association, Melbourne,
VIC, 2004. • State of California Department of Transport (Caltrans) Standard Specifications – Division V –
Section 39, Caltrans, 2015. • Arizona Department of Transportation (ADOT) Standard Specifications for Road and Bridge
Construction, ADOT, 2008. • AS 2150-2005 Hot mix asphalt a guide to good practice, Standards Australia Acknowledgements The development of this pilot specification is a result of a collaborative effort between representatives from state road agencies, the Australian Road Research Board, Tyre Stewardship Australia and industry. The AAPA National Technology and Leadership Committee especially acknowledges the contributions of the Queensland Department of Transport and Main Roads, Main Roads Western Australia, the Australian Research Board and the Queensland AAPA Technical Committee.
Disclaimer Although the information in this specification guide is believed to be correct at the time of printing, the Australian Asphalt Pavement Association, and agents of that organisation together with individuals involved in the preparation of this specification guide do not accept any contractual, tortious or other form of liability for its contents or any consequences arising from its use. People using the information contained in this guide should apply, and rely upon, their own skills and judgement to the particular issue they are considering. Suggestions for improvements are welcomed, please forward suggestions to the AAPA head office. Contact details available at aapa.asn.au.
Page | 2 Crumb Rubber Modified Open Graded and Gap Graded Asphalt Pilot Specification
1. General 1.1. Scope
This pilot specification sets out the requirements for crumb rubber modified (CRM) open graded asphalt (OGA) surface layers with a nominal maximum aggregate size of 10 mm and 14 mm. The specification also includes requirements for CRM gap graded asphalt (GGA) mixes with a nominal maximum aggregate size of 14 mm and 20 mm. The specification covers: • Constituent materials • OGA and GGA mix design requirements • Process control in manufacture and placement of asphalt • Acceptance criteria for the finished CRM asphalt pavement • Quality systems, minimum process standards, plant requirements and sampling and testing
1.2. Quality system requirements The Contractor shall establish, implement and maintain a Quality System in accordance with this Specification and the requirements of AS/NZS ISO 9001, or an equivalent system approved by the Principal. The Quality System shall include the appropriate Occupational Health and Safety procedures and Safe Working Method Statements. Where required in the Contract general clauses, the Contractor shall submit a Quality Plan prior to commencement of any works. The Quality Plan shall take into account the specific requirements for inspection and testing, acceptance/rejection criteria, details of proposed methods and other quality requirements that are contained in the Contract Documents. No part of the Quality System shall be used to pre-empt or otherwise negate the technical requirements of the Contract Documents.
1.3. Testing requirements
All testing of properties required by this Specification shall be undertaken in a laboratory accredited by the National Association of Testing Authorities (NATA) or International Accreditation New Zealand (IANZ) for the appropriate tests and performed in accordance with procedures contained in the relevant Australian Standard or Austroads Manual of Test Procedures. Where there is no applicable Australian Standard or Austroads Test Method, or where the Standard/Manual provides a choice of procedures, the method to be adopted shall be agreed between the Principal and the Contractor.
1.4. Defect liability period During the first 12 months, the product must not rut, shove, strip, ravel or bleed.
2. Constituent materials
2.1. Aggregate & mineral filler 2.1.1. General
All aggregates shall be obtained from established quarries and have established properties. Each individual aggregate fraction shall be obtained from the same quarry as the materials used in the design of the Job Mix. An appropriate system of stockpile management shall be implemented at the quarry and asphalt plant to ensure contamination does not occur. All mineral filler shall come from established sources and have established properties.
2.1.2. Coarse aggregate
Coarse aggregate is comprised of crushed rock particles that are substantially retained on the 4.75 mm sieve. Coarse aggregate shall comply with Australian Standard AS 2758.5 with the application of those test properties specified in Table 2-1 as appropriate.
Page | 3 Crumb Rubber Modified Open Graded and Gap Graded Asphalt Pilot Specification
Table 2-1: Coarse aggregate requirements
Property Test Method Requirement Particle size distribution (PSD) AS 1141.11.1 Report Crushed particles (1) AS 1141.18 100% crushed aggregate Polished aggregate friction value (PAFV) AS 1141.40, or AS 1141.41 ≥ 48 (2)
Particle density (Dry basis) AS 1141.6.1, or AS1141.6.2 report Water absorption AS 1141.6.1, or AS1141.6.2 ≤ 2.5 % Los Angeles abrasion loss (3) AS 1141.23 ≤ 25 % Ten percent fines value (wet) (3) AS 1141.22 ≥ 150 kN Wet/dry strength variation (3) AS 1141.22 ≤ 35 % Flakiness index AS 1141.15 ≤ 25%
Notes: 1. Test only required on river gravels and metasediments 2. In some regions aggregates that comply with the PAFV requirements in Table 2-1 may not be available. Where
this is the case, a lower PAFV requirement may be proposed for acceptance by the Principal. 3. Aggregate to be tested for either Los Angeles abrasion loss, or wet strength and wet/dry strength variation
2.1.3. Fine aggregate
Fine aggregate shall consist of crushed rock particles substantially passing the 4.75 mm sieve and manufactured from an approved source complying with the requirements of Section 2.1.2. The fine aggregate shall be clean, hard, durable and free from lumps of clay and other aggregations of fine materials, organic material and any other deleterious material. Fine aggregate shall comply with the criteria in Table 2-2.
Table 2-2: Fine aggregate requirements
Property Test Method Requirement Particle size distribution (PSD) AS 1141.11.1 Report Particle density (Dry basis) AS 1141.5 Report Water absorption AS 1141.5 ≤ 2.5 % Degradation Factor, Crusher fines (1) AS 1141.25.3 ≥ 60 Sodium Sulfate Soundness (weighted loss) (1) AS 1141.24 ≤ 12%
Notes: 1. Aggregate to be tested for either degradation factor, or Sodium Sulfate Soundness
2.1.4. Mineral filler
Mineral filler is that portion of mineral matter passing a 0.075 mm sieve, and includes rock dust derived from coarse and fine aggregates used in the production of asphalt in accordance with this specification, and any other materials added to supplement the quantity and properties of filler in the mix. OGA shall contain hydrated lime, or adhesion agent. Where hydrated lime is used a minimum of 1.0% shall apply. The combined filler shall comply with the requirements in Table 2-3
Page | 4 Crumb Rubber Modified Open Graded and Gap Graded Asphalt Pilot Specification
Table 2-3: Combined filler requirements
Property Test Method Requirement Voids in dry compacted filler AS/NZS 1141.17 ≥ 28 %
and ≤ 45 %
Apparent density of filler AS/NZS 1141.7 Report Methylene blue test1 AS 1141.66 ≤ 182
≤ 103 Notes: This requirement shall only apply for aggregate from New South Wales or Queensland. This requirement shall apply on the combined filler in asphalt (excluding hydrated lime) 3.Where meth